COPPER-PLATED STAINLESS STEEL FOR BIPOLAR PLATES IN DIRECT-OXIDATION SOFC
INTRODUCTION • Direct oxidation of dry hydrocarbon in SOFC • CeO2, Cu catalyst in anode • 700oC • Gas-tight seals for an SOFC with a Cu-based anode in a stainless-steel bipolar plate • Carbon formation is prevented when the steel is electroplated with a thin Cu film. • Basic study for large scale stack and multi-stacking
Double casting and calcined at 1550oC for; Porous Anode: 2.5 2.5 cm2 , 600m 10 wt% Ceria, 20wt% Cu as catalyst Poreformer : PMMA, Graphite electrolyte: 90 m Cathode: LSM (La0.8Sr0.2MnO3) + YSZ calcined at 1250oC 1~3 cm2 Cell holder: 430 Stainless steel Fuel channel made by CNC machine sealing: Commercial Ceramic sealing Copper plating on fuel channel by using copper Sulfate bath To prevent catalytic carbon deposition formed by Ni, Fe in stainless steel Analysis for carbon deposition GCMS Series connection of fuel between two cell for high conversion 5 3 4 6 6 2 1 1: Stainless steel stack 2: Cu-cermet anode 3: Electrolyte 4: Cathode 5: Pt current collector 6: Ceramic seal Experiment Schematic diagram of the SOFC mount used in this study.
V-i Curves & AC-Impedance Analysis Cell potential and power density vs. current density while running on H2 and n-butane at 973 K. The squares are for H2 and the circles for n-butane. Power density : 0.16W/cm2 for H2, 0.09W/cm2 for butane
Cell performance in n-butane as a function of time at 973 K while holding the cell potential at 0.5 V. Very stable performance during 90 hours Long Run Test for Hydrocarbon
Photograph of cell mount before (a) and after (b) exposure to n-butane at 973 K for24 hrs. Copper plating on Fuel Channel for reducing the catalytic carbon deposition enduced by Ni, Fe in stainless steel Thin carbon deposition on Copper layer after test Easily removed by toluene and analyzed by GCMS (b) (a) Before and After Test
Table 1. Names and molecular weights for selected products that are shown in Figure Analysis for Carbon Deposition • The GC trace obtained from the carbonaceous deposits formed on Cu-plated stainless steel following exposure to n-butane at 973 K for 24 hours. • The structures of selected species are given, along with numbers corresponding to the compounds in Table 1. • Poly-Aromatic Hydrocarbons (PAHs) with 2~6 benzene rings
2-series connection High conversion of fuel OCV 2.1V for H2 1.9V for butane Power density 0.29 W/cm2 for H2 0.16 W/cm2 for butane H2 butane Cathode Fuel Anode Cathode High conversion Anode Multi-Stage Connection for High Conversion
Conclusion • It is possible to obtain gas-tight seals for an SOFC with a Cu-based anode in a stainless-steel bipolar plate • The tar-like substances on Cu plating analyzed by GC-MS consist primarily of poly-aromatic hydrocarbons having between 2~6 aromatic rings.These compounds are probably form as a result of gas-phase, free-radical reactions. It is important to note that these deposits are very different from what is formed in the presence of a metal catalyst such as Ni or Fe. • The series-fuel providing to multi-stage cells can increase the conversion and efficiency of fuel.